Section 2: Purchasing Instructions
2.6 Welding Practices
Background information regarding welding and associated temperature control of Grade 91 steel is given in Appendix G and the 2015 EPRI report, A Perspective on the Selection of Preheat, Interpass and Post-Weld Cool Temperatures Using Grade 91 Steel as an Example (3002005351) . It must be strongly recommended that qualification and use of solid wire gas metal arc welding (GMAW) should be approached with caution. The current Grade 91 (-B9) composition is lean on deoxidizing elements (such as Mn and Si). These elements are important to proper operation and results with GMAW. Because of this, wetting action is reduced and the preponderance for lack of fusion type defects and oxide inclusion content affect the ability to perform successful welding. A few fabricators have qualified GMAW but under very controlled conditions and in some cases with compositions that provide adequate deoxidizers. Few organizations have properly and effectively implemented the solid-wire GMAW process for field installation or repairs.
2.6.1 Preheat and Interpass Temperature
A variety of methods are available, and it is mandatory to control the minimum preheat temperature, as follows:
For welds made using the flux-cored arc welding (FCAW) process or the submerged arc welding (SAW) process or in a highly restrained component, a minimum preheat temperature of 400°F (205°C) shall be maintained.
For welds made using the shielded metal arc welding (SMAW) process, a minimum preheat temperature of 300°F (150°C) shall be maintained until the welding is complete.
For welds made using either the GMAW process or the gas tungsten arc welding (GTAW) process with a solid wire filler metal, a minimum preheat temperature of 300°F (150°C) shall be maintained until the welding is complete.
For welds made using either GMAW or GTAW with a filler metal other than solid wire (that is, metal-cored or flux-cored), a minimum preheat temperature of 300°F (150°C) shall be maintained. An exception to this rule shall apply for welds that effectively are self-preheating—that is, welds involving a relatively small heat sink in comparison with the magnitude of the arc energy or heat input and that are continuously deposited so that the entire weld nugget and base metal HAZ remain above the specified minimum preheat level throughout the weld cycle.
If welding is interrupted, preheat temperature must be maintained. Although not a recommended practice, if the joint temperature drops below the preheat temperature, the interrupted welds must be as follows:
At least one-third of the final through-wall thickness of the component
Given a hydrogen bake before slow cooling to room temperature
Kept dry until the welding is re-started with the proper preheat
These precautions are necessary because, in the as-welded condition, the joint can be vulnerable to SCC. Appendix F details additional information on stress corrosion susceptibility in Grade 91.
The maximum interpass temperature during welding shall be 660°F (350°C).
2.6.2 Hydrogen Bake
Following welding, if there is a need for the temperature of the weld to be dropped to room temperature prior to the implementation of the PWHT, to control the amount of diffusible hydrogen present in the weldments, a hydrogen bake should be performed. The hydrogen bake involves holding in the
temperature range of 500°F–660°F (260°C–350°C) for 1 hour minimum for thicknesses of 1 in. (25.4 mm) or less and 2 hours for thicknesses greater than 1 in. (25.4 mm). If it is certain that low hydrogen practices have been successful in limiting the amount of hydrogen in the weldment, a hydrogen bake is not necessary, but this is still considered good practice.
2.6.3 Post-Weld Heat Treatment
Following completion of welding, the temperature of the component should be allowed to cool to at the least the specified preheat temperature, provided that this value is ≤400°F (205°C). Where there is specific concern of temperature inhomogeneity through the thickness of the weldment, lower post-weld cool temperatures should be considered according to the information provided in EPRI report 3002005351 .
The component should be post-weld heat-treated within 8 hours of the completion of welding. If this is not possible, either the component should be maintained at a minimum temperature of 175°F (80°C) or the humidity of the environment in which the weld is stored should be controlled to guarantee that no condensation can occur at any time (for example, because of changes in temperature) on either the outer diameter (OD) or inner diameter (ID) surfaces of the joint until the PWHT can be initiated.
An agreement between client and contractor should be established on the best practice to minimize the risk of SCC occurring on any Grade 91 components (see Appendix F for more information).
The PWHT should be performed within the range of 1247°F–1418°F (675°C–
770°C). The maximum temperature at any point in the PWHT process should not exceed 1418°F (770°C). The minimum temperature is recommended based on EPRI research . The maximum temperature differs from the
requirements stated in ASME Section I for P15E materials where the stated maximum is dependent on composition, as follows:
If Ni+Mn is ≤1.0 wt%, the maximum is 1470°F (800°C).
If Ni+Mn is >1.0 but <1.2 wt%, the maximum is 1445°F (785°C).
If the Ni+Mn content of the filler material is not known, the maximum PWHT temperature is 1445°F (785°C).
The reduced maximum PWHT temperature of 1418°F (770°C) provides a buffer during PWHT to minimize the risk of undesirable metallurgical transformations.
Information on control of the PWHT within the defined limits is provided in Appendix C. The temperature and time at temperature for the PWHT should be selected to ensure that the hardness at all locations in the area heated is within the specified range.
No additional limits on the rate of heat-up or cooldown are specified for PWHT.
However, for thick-walled components, or for assemblies of complex shape, an appropriate rate of heat-up or cooldown, as determined by experienced engineering judgment, should be adopted to minimize distortion and residual stresses.
Note: Prior to the application of the PWHT to Grade 91 welds, the weld metal and portions of the HAZ are vulnerable to brittle fracture if subjected to abnormally high mechanical loads during handling. Care shall be taken, therefore, in the handling of Grade 91 weldments in the as-welded condition to minimize the risk.
2.6.4 Filler Materials
188.8.131.52 Matching Filler Metal
Matching filler materials that have similar chemistry and strength to the base metal should be used for all joints between Grade 91 materials. Insofar as it is possible, the chemical composition of the matching filler metal shall conform to the elemental restrictions specified in Table 2-2.
Recommended chemical composition requirements for Grade 91 matching filler materials
Elements1,2,3 SMAW Electrodes GMAW/GTAW Bare,
SAW (Weld Deposit
Wire/Flux Combination) FCAW Electrodes
C 0.08–0.13 0.07–0.13 0.07–0.13 0.08–0.13
(0.04–0.07) (0.04–0.07) 0.03–0.07